This preview has intentionally blurred sections. Sign up to view the full version.
View Full DocumentThis preview has intentionally blurred sections. Sign up to view the full version.
View Full Document
Unformatted text preview: ,J‘ LOUISIANA STATE UNIVERSITY Mechanical Engineering Department
Professor Meletis ME 2733 Spring 2004
Midterm Examination
Name:
(40 P18) 1. State ifthefollowing statementsaretrue ('I')orfalse (F).
(a) In general, BCC metals exhibit a ductilebrittle transition. T (b) High ﬁacttue toughness requires moderate strength and moderate ductility. T
(c) Dislocations require less energy to move in FCC compared to BCC metals. T
(d) The BCC metal W is closed packed. T (emmateﬁalwimadeepepomﬁal wellhashighmelﬁngpointbmlowmodulus. T (0 Cr is a BCC metal and;xhibits {iiiTraction for the (31 i) plane. T
(g) A screw dislocation is a point defect. T
(h) Recrystallization causes an increase in ductility and strength. T
(i) Doping Si with A1 creates a p—type semiconductor. T (j) Semiconductors have higher conductivity than metals. T . I. (20 p18) ‘ .
2. A cylindrical metal rod, 5 inches long and with a Imiform crosssectional area of 0.01 inz, is
f loaded in tension.
First, a load of2,000 lbs is applied and the rod becomes 5.005 inches long. Whenthe load is
released, therod goesbaekto its original lengthofs inches. Themmerod is]oadeda15,0001bsandafterﬂ1atis mloaded.Aﬁe1mﬂoedingthetotal lengthof
the rod is 5.01 inches. (:0 Calculate the elastic modulus of the material. (b) Calculate the engineering strain after unloading the rod ﬁ'om 5,000 lbs. (1:) Calculate the true strain after unloading the rod ﬁom 5,0001be. ' ((1) Determine the yield strength ofthe material. ' .9" (20m)
3. AsanneyouaddCrmdNto Fetocremiemsolidsolutions:onewitl10.2atomic%Crandﬂ1e second with 0.2 atomic % N. (a) What type of solid solutions are they?
Fe0.5%Cr:
Fe0.5%N: (b) Compmthediﬂ’usiﬁtiesofCrinFeandCinFe. Whichoneishigher‘? DCrinFe 01‘ DNinFe (c) What is the meclnnism of diffusion for your selection in (b)? (d) Which solidsolution do you expect to have higher strength?
FeO.S%'Cr or Fe0.5%N (e) Do you expect any signiﬁcant change in the eiasﬁc modulus of Fe by adding Cr orN? Yes or No in m 9")
‘ 4. The hypothetical metallic elements A and B form the crystal structure shown below. (a) What is the Bravais lattice? (b)HowmanyAandBanmsareassociataedpqlatﬁcepoint? A:_ B: (c} How manyatoms arethere per unit cell?
(d)Whatdoyouexpecttheslipsystemtobeforﬂzis structure? Slip plane: ; Slip direction: (e) Calculate the theoretical density of this material. (Atomic weights A: 340; B: 300) ...
View
Full Document
 Fall '10
 Meng

Click to edit the document details